General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.1 g/cm³ Show Material materials with Density of 8.1 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa |

100.0 °C | 201 GPa Show Material materials with Elastic modulus of 201 GPa | |

200.0 °C | 196 GPa Show Material materials with Elastic modulus of 196 GPa | |

300.0 °C | 191 GPa Show Material materials with Elastic modulus of 191 GPa | |

400.0 °C | 186 GPa Show Material materials with Elastic modulus of 186 GPa | |

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | |

600.0 °C | 171 GPa Show Material materials with Elastic modulus of 171 GPa | |

700.0 °C | 161 GPa Show Material materials with Elastic modulus of 161 GPa | |

800.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

900.0 °C | 138 GPa Show Material materials with Elastic modulus of 138 GPa | |

1000.0 °C | 129 GPa Show Material materials with Elastic modulus of 129 GPa | |

1100.0 °C | 130 GPa Show Material materials with Elastic modulus of 130 GPa | |

Elongation | 20.0 °C | 30 % Show Material materials with Elongation of 30 % |

Hardness, Brinell | 20.0 °C | 220 [-] Show Material materials with Hardness, Brinell of 220 [-] |

Tensile strength | 20.0 °C | 550 - 750 MPa Show Material materials with Tensile strength of 550 - 750 MPa |

Yield strength Rp0.2 | 20.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2 of 205 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.38E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.38E-5 1/K | |

200.0 °C | 1.44E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.44E-5 1/K | ||

300.0 °C | 1.46E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.46E-5 1/K | ||

400.0 °C | 1.48E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.48E-5 1/K | ||

500.0 °C | 1.51E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.51E-5 1/K | ||

600.0 °C | 1.57E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.57E-5 1/K | ||

700.0 °C | 1.63E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.63E-5 1/K | ||

800.0 °C | 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.67E-5 1/K | ||

900.0 °C | 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.72E-5 1/K | ||

1000.0 °C | 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.77E-5 1/K | ||

1100.0 °C | 1.83E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.83E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 1200 °C Show Material materials with Max service temperature, long of 0 - 1200 °C | ||

Melting point | 1200 - 1480 °C Show Material materials with Melting point of 1200 - 1480 °C | Typical for Nickel Chromium Iron Alloy | |

Specific heat capacity | 20.0 °C | 450 J/(kg·K) Show Material materials with Specific heat capacity of 450 J/(kg·K) | |

100.0 °C | 470 J/(kg·K) Show Material materials with Specific heat capacity of 470 J/(kg·K) | ||

200.0 °C | 500 J/(kg·K) Show Material materials with Specific heat capacity of 500 J/(kg·K) | ||

300.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

400.0 °C | 550 J/(kg·K) Show Material materials with Specific heat capacity of 550 J/(kg·K) | ||

500.0 °C | 580 J/(kg·K) Show Material materials with Specific heat capacity of 580 J/(kg·K) | ||

600.0 °C | 600 J/(kg·K) Show Material materials with Specific heat capacity of 600 J/(kg·K) | ||

700.0 °C | 630 J/(kg·K) Show Material materials with Specific heat capacity of 630 J/(kg·K) | ||

800.0 °C | 660 J/(kg·K) Show Material materials with Specific heat capacity of 660 J/(kg·K) | ||

900.0 °C | 690 J/(kg·K) Show Material materials with Specific heat capacity of 690 J/(kg·K) | ||

1000.0 °C | 710 J/(kg·K) Show Material materials with Specific heat capacity of 710 J/(kg·K) | ||

1100.0 °C | 740 J/(kg·K) Show Material materials with Specific heat capacity of 740 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 11.3 W/(m·K) Show Material materials with Thermal conductivity of 11.3 W/(m·K) | |

100.0 °C | 12.7 W/(m·K) Show Material materials with Thermal conductivity of 12.7 W/(m·K) | ||

200.0 °C | 14.4 W/(m·K) Show Material materials with Thermal conductivity of 14.4 W/(m·K) | ||

300.0 °C | 16 W/(m·K) Show Material materials with Thermal conductivity of 16 W/(m·K) | ||

400.0 °C | 17.6 W/(m·K) Show Material materials with Thermal conductivity of 17.6 W/(m·K) | ||

500.0 °C | 19.2 W/(m·K) Show Material materials with Thermal conductivity of 19.2 W/(m·K) | ||

600.0 °C | 20.6 W/(m·K) Show Material materials with Thermal conductivity of 20.6 W/(m·K) | ||

700.0 °C | 22.2 W/(m·K) Show Material materials with Thermal conductivity of 22.2 W/(m·K) | ||

800.0 °C | 24.5 W/(m·K) Show Material materials with Thermal conductivity of 24.5 W/(m·K) | ||

900.0 °C | 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26.1 W/(m·K) | ||

1000.0 °C | 27.7 W/(m·K) Show Material materials with Thermal conductivity of 27.7 W/(m·K) | ||

1100.0 °C | 29.3 W/(m·K) Show Material materials with Thermal conductivity of 29.3 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m |

100.0 °C | 1.2E-6 Ω·m Show Material materials with Electrical resistivity of 1.2E-6 Ω·m | |

200.0 °C | 1.22E-6 Ω·m Show Material materials with Electrical resistivity of 1.22E-6 Ω·m | |

300.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

400.0 °C | 1.25E-6 Ω·m Show Material materials with Electrical resistivity of 1.25E-6 Ω·m | |

500.0 °C | 1.25E-6 Ω·m Show Material materials with Electrical resistivity of 1.25E-6 Ω·m | |

600.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

700.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

800.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

900.0 °C | 1.28E-6 Ω·m Show Material materials with Electrical resistivity of 1.28E-6 Ω·m | |

1000.0 °C | 1.29E-6 Ω·m Show Material materials with Electrical resistivity of 1.29E-6 Ω·m | |

1100.0 °C | 1.3E-6 Ω·m Show Material materials with Electrical resistivity of 1.3E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 1 - 1.7 % Show Material materials with Aluminium of 1 - 1.7 % |

Boron | 6E-3 % Show Material materials with Boron of 6E-3 % |

Carbon | 0.03 - 0.1 % Show Material materials with Carbon of 0.03 - 0.1 % |

Chromium | 21 - 25 % Show Material materials with Chromium of 21 - 25 % |

Copper | 0.5 % Show Material materials with Copper of 0.5 % |

Iron | 18 % Show Material materials with Iron of 18 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Nickel | 58 - 63 % Show Material materials with Nickel of 58 - 63 % |

Phosphorus | 0.02 % Show Material materials with Phosphorus of 0.02 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.5 % Show Material materials with Titanium of 0.5 % |